  The study establishes that the degree of optically induced spin polarization
that can be achieved for NV$^- $in 1b diamond is limited by the concentration
of single substitutional nitrogen, N$^0$ . The polarization of the individual
NV centres in the diamond is dependent on the separation of the NV$^-$ and the
nitrogen donor. When the NV$^-$ - N$^+$ pair separation is large the properties
of the pair will be as for single sites and a high degree of spin polarization
attainable. When the separation decreases the emission is reduced, the lifetime
shortened and the spin polarization downgraded. The deterioration occurs as a
consequence of electron tunneling in the excited state from NV$^-$ to N$^+$ and
results in an optical cycle that includes NV$^0$. The tunneling process is
linear in optical excitation and more prevalent the closer the N$^+$ is to the
NV$^-$ centre. However, the separation between the NV$^-$ and its donor N$^+$
can be effected by light through the excitation of NV$^-$ and/or ionization of
N$^0$. The optical excitation that creates the spin polarization can also
modify the sample properties and during excitation creates charge dynamics. The
consequence is that the magnitude of spin polarization, the spin relaxation and
coherence times T$_1$ and T$_2$ have a dependence on the nitrogen concentration
and on the excitation wavelength. The adjacent N$^+$ gives an electric field
that Stark shifts the NV$^-$ transitions and for an ensemble results in line
broadening. It is observation of changes of these Stark induced effects that
allow the variation in NV$^-$ - N$^+$ separation to be monitored. Spectroscopic
measurements including that of the varying line widths are central to the
study. They are made at low temperatures and include extensive measurements of
the NV$^-$ optical transition at 637 nm, the infrared transition at 1042 nm and
ODMR at 2.87 GHz.
